Self-cooling by ferrofluid in magnetic field
- 103 Downloads
This paper reports the synthesis of Fe3O4 ferrite nanoparticles and ferrofluid via a coprecipitation method. Structural studies were investigated using X-ray diffraction technique that confirmed the formation of single-phase cubic spinel structure. Morphology and particle size were elucidated using high-resolution transmission electron microscopy. Magnetic characteristics were investigated using a vibrating sample magnetometer, and saturation magnetization of nanoparticles was found to be 23.72 emu/gm with negligible coercivity and retentivity showing superparamagnetic behaviour. A functional self-cooling design employing ferrofluid (as a coolant) was demonstrated in which the system uses heat from the heat source and a permanent magnet to maintain the fluid flow that transfers heat to heat sink. The system is self-regulating and requires no power or pump for flowing of the fluid in the loop. The performance of the device on various parameters like volume fraction of nanoparticles, the temperature of heat source and strength of the magnetic field has also been studied. It was found that cooling by ~ 20 °C was achieved when temperature of heat source was maintained at 85 °C. Cooling performance was enhanced by ~ 7% when the concentration of nanoparticles in ferrofluid was increased from 2 to 6% and by ~ 4% upon the application of magnetic field.
KeywordsFerrofluid Heat transfer Nanoparticles Coprecipitation method Magnetic field
The cooling operation of many industrial systems is restricted by using traditional heat transfer fluids such as water, kerosene and ethylene glycol, which have poor thermal conductivity. By substituting these with higher thermal conductivity fluids, the performance of such devices can be improved. Choi , by adding nanoparticles to the fluids, presented an innovative way to improve their thermal conductivity. Suspending nanoparticles in a suitable carrier liquid alters the flow and heat transfer properties of the base fluid. Li et al. investigated the thermophysical properties of nanofluids of silver and single-walled carbon nanotubes by dispersing them in distilled water. They suggested that some nanofluids with suitable thermophysical properties can be used in the refrigeration system as the secondary working fluids in condenser . Sarafraz et al. conducted a study to evaluate the efficiency and thermal performance of solar collector employing graphene-methanol nanofluids in heat pipes. It was found that graphene nanoplatelets enhanced the thermal conductivity of methanol by 20% . Goodarzi et al. carried out a numerical study on the free convection of water-based nanofluids with Al2O3, Cu and multi-walled carbon nanotubes nanoparticles inside a closed cavity. They showed that density difference due to temperature gradient has a great effect on fluid circulation and hence heat transfer in the cavity . Jalali et al. presented a numerical study of laminar flow and nanofluid jet injection of oil-based multi-walled carbon nanotube nanofluid in a microchannel. It was found that dispersing the solid nanoparticles in oil with a higher concentration and using nanofluid jet injection increased the rate of heat transfer by disturbing the thermal boundary layer . Hassan carried out a comparative study on a series of nanofluid with magnetic and non-magnetic particles. They showed that although nanofluid with non-magnetic particles has a higher thermal conductivity than nanofluids with magnetic nanoparticles, the heat transfer rate is faster in magnetic nanofluid due to the applied magnetic field which can control the rate of heat transfer. Further, the heat transfer rate is enhanced by increasing the nanoparticles concentration and reducing the particle size . Marin et al. examined the hydromagnetic transport of Fe nanoparticles suspended in water. They showed that the rate of heat transfer can be enhanced by increasing the concentration of nanoparticles in the back bone. However, increasing the dead-end particles improved the wall shear stress and decreased the rate of heat transfer . Hassan et al. investigated the flow of ferrofluid over a rotating disc in the oscillating magnetic field. They found that when compared to zero-field condition, the particles rotate faster and the viscosity of ferrofluid is reduced, leading to enhanced heat transfer rate under an oscillating magnetic field . Many other studies have been carried out investigating the role of nanofluids in the heat transfer rate [9, 10, 11, 12, 13].
Ferrofluids are colloidal suspension of magnetic nanoparticles in the magnetically passive carrier liquid. The nanoparticles are layered with a surfactant to maintain a stable state. However, due to dipole–dipole interactions and van der Waals forces between the magnetic nanoparticles, they may combine to form agglomerations at a high concentration. Without magnetic field, nanoparticles are oriented randomly, whereas, with magnetic field, they align in the applied field direction .
Many thermal management systems employing liquid cooling technology have been successfully used in various electronic devices. However, most of these techniques have drawbacks such as vibrating moving parts, noise problem, leakage, high maintenance and large power consumption due to driving pump [15, 16, 17]. From the last several decades, researchers have proposed liquid transport systems without pumps to overcome the aforementioned problems. Membrane structure-based actuators have been proposed like piezoelectric, magnetic, shape-memory alloy and thermo-pneumatic actuators [18, 19, 20, 21]. However, considering the fluctuations in temperature and pulsating flow, they are not considered reliable.
In recent years, ferrofluid has fascinated many researchers in cooling application due to enhanced heat transfer characteristics. Experimental investigations show that the enhancement in heat transfer properties mainly depends on various parameters like volume fraction, size, chemical composition of nanoparticles, temperature of heat source, strength of magnetic field and base fluid. Many researchers in the past have investigated on heat transfer characteristics of ferrofluid in natural convection and reported the enhancement in heat transfer, making them suitable for cooling applications [22, 23]. Lajvardi et al. built an experimental set-up to study the heat transfer characteristics of ferrofluid in a heated copper tube. It was found that heat transfer is significantly enhanced by applying the magnetic field and by increasing the concentration of nanoparticles in ferrofluid. This enhancement was attributed to the improved thermophysical properties of ferrofluid . Bahiraei et al. carried out a numerical investigation on water-based Fe3O4 ferrofluid in a square channel under the applied magnetic field. They studied the effect of various factors like concentration and diameter of nanoparticles, strength of magnetic field and Reynolds number. It was established that increasing the strength of magnetic field and using ferrofluid with a higher nanoparticle concentration and diameter lead to the enhancement in the heat transfer rate . Wen et al. constructed an experimental system to study the heat transfer properties of nanofluids and asserted that the use of nanofluids significantly improved the heat transfer in the laminar flow regime, which was due to the migration of particles, resulting in higher thermal conductivity, and reduced the thickness of thermal boundary layer . Li et al. established a miniature cooling device using ferrofluid and investigated its operational characteristics. They showed that the flow velocity of the ferrofluid increases on increasing the temperature of heat load, applying stronger magnetic field which enhances the performance of cooling device .
In this paper, Fe3O4 ferrite/ferrofluid has been prepared by a coprecipitation method. Structural, morphological and magnetic properties of developed nanoparticles have been studied using XRD, HRTEM and VSM. An automatic cooling device is constructed employing Fe3O4–kerosene ferrofluid, owing to their long-term stability. By analysing the experiments performed, the effect of concentration of nanoparticles in ferrofluid, magnetic field (external) and temperature of heat source on the efficiency of the cooling device is investigated and discussed.
2 Materials and methods
The synthesis of Fe3O4–kerosene-based ferrofluid involves mainly two steps: synthesis of Fe3O4 nanoparticles and dispersing them in a suitable carrier liquid, i.e. kerosene to get a stable ferrofluid. Fe3O4 nanoparticles were prepared by the chemical coprecipitation technique using analytical-grade chemical reagents (Sigma-Aldrich). In the process, iron(II) chloride (FeCl2) and iron(III) chloride (FeCl3) were chosen as initial precursors in the ratio (Fe2+/Fe3+) 1:2. Each of these was mixed separately with distilled water in appropriate molar quantities to get a homogeneous solution. These salt solutions were then mixed and stirred, while oleic acid was added dropwise to the solution to prevent their agglomeration. Later, under vigorous stirring and constant heating at 80 °C, analytical-grade ammonia (NH3) solution was put dropwise for immediate precipitation. The pH of the reaction mixture was monitored constantly, and ammonia was added until its pH reached 11. The nanoparticles obtained were washed several times with distilled water. Then, these samples were dispersed in suitable liquid (kerosene) and decanted to get a stable ferrofluid. The developed nanoparticles were spherical in shape with the diameter of 15–18 nm. Ferrofluid with different concentrations of nanoparticles, i.e. 2%, 4% and 6%, was prepared to carry out the study.
Synthesized nanoparticles were characterized on Rigaku Ultima-IV X-ray diffraction (XRD) having CuKα radiations at a scan rate of 2°/min for structural studies. Morphological studies were carried out using a high-resolution transmission electron microscopy (HRTEM) of Tecnai G2 20 (FEI) S-Twin at 200 kV. Magnetic studies were performed using Lakeshore VSM Model 7410 in the field range of ± 15,000 Gauss.
2.2 Experimental set-up for cooling
Here, when ferrofluid in the loop comes in the thermal field of heat source maintained at a constant temperature, fluid heats up, rises (some thermal energy gets converted to kinetic energy), move towards the sink and consequently transfers the heat from source to sink. After losing the heat to sink, this cold ferrofluid progresses towards heat source and the cycle goes on without employing any pump. The permanent magnet induces a driving force that allows a higher convective heat transfer rate. So, the driving force, which is responsible for circulating the fluid, depends upon magnetic field and temperature. After some time, if all the conditions are kept unchanged, then loop temperature stops increasing and eventually become constant, when it attains the thermal stability. This device is self-regulating, is easy to handle and requires no maintenance using the heat from heat source (e.g. boiling water, heat-dissipated electronic devices, etc.) as a driving force for liquids and reliable in the field of cooling. The cooling efficiency of the device is affected by the temperature of the source, concentration of nanoparticles and external magnetic field as discussed below.
3 Results and discussion
3.1 XRD analysis
The interplanar spacing and lattice parameter for the synthesized sample was calculated as 2.52 Å and 8.35 Å, respectively, which are in good agreement with the standard data. The sample showed broad peaks, signifying the fine and small crystallite size; therefore, ferrofluids can be easily synthesized by making use of the small size of the particles.
3.2 HRTEM analysis
3.3 VSM analysis
The saturation magnetization value for Fe3O4 nanoparticles depends upon superexchange interaction and particle size. The smaller the size is, the lesser the magnetization of the particle will be due to prominent surface effects in the nanoparticles due to spin canting disorder on the surface, since the surface-to-volume ratio increases significantly in nanoparticles and their surface is composed of some canted spins that prevent the core spins to align in the direction of magnetic field, hence decreasing their saturation magnetization [31, 32, 33].
4 Experimental set-up
4.1 Role of temperature of the heat source
4.2 Role of concentration of nanoparticles
At low concentration of nanoparticles (2%), enhancement observed in heat transfer may be attributed to the following effects: (a) thermoconvection of fluid and (b) Brownian motion caused by the random motion of dispersed nanoparticles due to collision among themselves and with molecules of the base fluid. In thermoconvection, when the fluid enters the thermal field of source, it begins to rise towards the sink. Further, Brownian motion contributes to the enhancement in the rate of heat transfer in further two ways: first, by direct influence of diffused nanoparticles that transport heat and second, by indirect influence by microconvection of the base fluid .
At higher concentration, properties of the ferrofluid are influenced by interparticle interactions, as a result of chainlike structures formed due to dipole interactions among magnetic nanoparticles; however, Brownian motion becomes negligible. So, when the concentration of nanoparticles in ferrofluid increases, dipolar interaction becomes stronger and starts to form chainlike aggregates of nanoparticles which transport heat more effectively . The formation of these chains in such a stable ferrofluid leads to highly conductive and lengthened path for the flow of heat that results in an increase in the rate of heat transfer, since solid particles conduct heat at a faster rate than the base fluid .
So, it can be noted from Fig. 6 that the cooling performance of the device is enhanced as the concentration of nanoparticles is increased from 2 to 6%. Asymptotic behaviour of the temperature in Fig. 6 can be understood as: here, the temperature of heat load was maintained at 75 °C, and when ferrofluid comes in its thermal vicinity, the temperature of the fluid in the system starts rising. Further, non-uniform temperature distribution and high temperature of heat load induce ferrofluid to circulate in the loop and transfer the heat from heat load to sink. The temperature of the system stops rising when thermal steady state is achieved. The temperature follows the same trend for all the volume fractions. Cooling performance is enhanced by 7% when the concentration of ferrofluid was increased from 2 to 6% due to increased interparticle interaction forming chainlike structures, which leads to highly conducting path for heat flow.
4.3 Role of magnetic field
Yarahmadi et al.  found out that the application of a constant magnetic field exerts an inverse effect on the convective heat transfer and causes the heat transfer to decline. Lajvardi et al.  found out that the use of Fe3O4 magnetic nanoparticles as the dispersed phase in water cannot enhance the convective heat transfer in the laminar flow regime in the absence of magnetic field. However, using our present device design, we have achieved cooling effects even in the absence of magnetic field, which increases even on the application of constant magnetic field. So, the drawbacks observed in earlier ferrofluid-based cooling device designs are removed in the present device. The studies carried by other researchers are on the role of device dependence on parameters like temperature gradient, heat load/sink temperature, role of AC or DC magnetic fields, etc., and their mathematical simulations [35, 41, 42]. Their studies are based on different experimental results and our present device design, and the results of measurements will surely add up for reaching to a good automatically cooling device using ferrofluids.
It is a self-powered, self-regulating device.
It does not require any pump or moving parts.
A variety of base fluids may be used as per requirement.
Extent of cooling can be controlled.
It is low cost.
It is easy to maintain and a reliable system.
However, with the advancement in nanotechnology and nanomaterials, such a cooling device proposed may find a better application where waste heat from electronic devices may be utilized.
Compliance with ethical standards
Conflict of interest
The authors declare that there is no conflict of interest.
- 1.Choi SUS, Eastman JA (1995) Enhancing thermal conductivity of fluids with nanoparticles. Dev Appl Non-Newton Flows 231:99–105Google Scholar
- 14.Rosensweig RE (1997) Ferrohydrodynamics. Dover Publications, New YorkGoogle Scholar
- 16.Fabbri M, Jiang S, Dhir VK (2005) A comparative study of cooling of high power density electronics using sprays and microjets. J Heat Transf 127:105–217Google Scholar
- 18.Shinozawa Y, Abe T, Kondo T (1997) A proportional microvalve using a bi-stable magnetic actuator. In: Proceedings of the 10th IEEE international workshop on MEMS, pp 233–237Google Scholar
- 26.Wen D, Ding Y (2004) Experimental investigation into convective heat transfer of nanofluids at the entrance region under laminar flow conditions. Int J Heat Mass Transf 47(24):5181–5188. https://doi.org/10.1016/j.ijheatmasstransfer.2004.07.012 CrossRefGoogle Scholar
- 28.Cullity BD (1978) Elements of X-ray diffraction. Addison-Wesley, ReadingGoogle Scholar
- 30.El Ghandoor H, Zidan HM, Khalil M, Ismail MIM (2012) Synthesis and some physical properties of magnetite (Fe3O4) nanoparticles. Int J Electrochem Sci 7:5734–5745Google Scholar